UNIVERSITA’ DEGLI STUDI DI PARMA
Dottorato di ricerca in Scienza e Tecnologia dei Materiali
Development of printed semiconducting gas sensors:
industrial, medical and environmental applications
Chiar.mo Prof. Enrico Dalcanale
Chiar.mo Ing. Antonino Bonanno
Chiar.ma Dott. Maria Cristina Carotta Chiar.mo Prof. Michele Sacerdoti
Dottorando: Ambra Fioravanti
In memory of Ing. Roberto Paoluzzi Director of CNR-IMAMOTER
TABLE OF CONTENTS
INTRODUCTION ... 1
CHAPTER 1: SEMICONDUCTING OXIDES GAS SENSORS: EXPERIMENTAL EVIDENCES AND RESPONSE MODELING ... 4
1.1 INTRODUCTION ... 4
1.2 EXPERIMENTAL EVIDENCES... 6
1.3 RESPONSE MODELING ... 13
CHAPTER 2: THICK FILM PREPARATION ... 22
2.1 INTRODUCTION ... 22
2.2 PREPARATION AND CHARACTERIZATION OF THE FUNCTIONAL MATERIALS ... 22
2.2.1 SYNTHESIS METHODOLOGY ... 24
2.2.2 CHARACTERIZATION OF THE FUNCTIONAL MATERIALS 25 2.2.3 SYNTHESIS PROCESSES ... 31
2.3 SCREEN-PRINTING PROCESS ... 35
2.4 ELECTRICAL LABORATORY CHARACTERIZATIONS ... 39
CHAPTER 3: SYNTHESIS OF ZNO NANOMORPHOLOGIES: STRUCTURAL AND ELECTRONIC PROPERTIES ... 43
3.1 INTRODUCTION ... 43
3.2 BASIC PROPERTIES ... 44
3.3 SYNTHESIS AND MORPHOLOGICAL CHARACTERIZATION OF ZNO NANOMORPHOLOGIES ... 46
3.3.1 MORPHOLOGICAL DEPENDENCE ON ZNO-PRECURSOR 51
3.3.2 STRUCTURAL CHARACTERIZATION ... 52
3.3.3 SPECTROSCOPIC CHARACTERIZATION ... 53
3.3.4 ELECTRICAL CHARACTERIZATION ... 55
3.3.5 SENSING PROPERTIES ... 57
CHAPTER 4: NOVEL METODOLOGIES FOR ON-LINE MONITORING THE HYDRAULIC OIL AGEING ... 62
4.1 INTRODUCTION ... 62
4.2 HYDRAULIC OIL SAMPLE COLLECTION: TEST BENCH ... 63
4.3 GAS CHROMATOGRAPHIC ANALYSIS ... 64
4.4 MOX SENSORS SYSTEM ... 66
4.5 ORGANIC ELECTROCHEMICAL TRANSISTORS (OETCs) ... 70
4.5.1 EXPERIMENTAL RESULTS ... 74
CHAPTER 5: MONITORING OF THE ATMOSPHERIC POLLUTANTS
GASES ... 77 5.1 INTRODUCTION... 77 5.2 REALIZATION AND CHARACTERIZATION OF THE MOX SENSOR
ARRAY ... 79 5.3 THE MONITORING UNIT ... 83 5.4 TEST IN FIELD THROUGH THE MONITORING UNITS ... 84
CONCLUSIONS ... 93
As a human being collects information about the surrounding environment with its senses, a sensor elaborates the signals perceived by a sensing element. However, while the reaction of a human being results into an emotional or intellectual behavior, the sensor only responds with analytical data.
The term “sensor” started to gain currency during the 1970s, and it identifies a transducer (or device) that detects and converts events or changes in its environment into data usefully observed or processed.
In principle, the input quantity measured and the output data provided can be of various type (chemical, electrical, magnetic, mechanical, thermal, radiant, etc.) making the sensors an essential tool both in scientific applications and in everyday life. Their development was mainly reinforced by technological improvements, in term of new nanostructured materials, microelectronics and miniaturization, and by the demand of real time, low cost and online devices. Over the years, the development of sensors for several applications ranging from micromechanics to medical diagnostics is so increased that the first decade of the 21st century has been labelled as “the sensor decade” .
The gas sensing application too is in great demand, to control a large variety of parameters such as environmental, food quality, biomedical, industrial process control, etc..
Nowadays there is a variety of structures, materials and working principles exploitable to realize gas sensors. Among them, semiconductor gas sensors using metal oxides (MOX) as gas sensing element are a convenient choice to detect a wide range of gases both in scientific research and in industrial applications. Although the metal oxides used as sensing materials have wide band gap typical of insulators, they possess conductivity in the range of semiconductors due to point defects in crystal structure. The gas sensing devices generally consist of a MOX semiconductor between two metal electrodes and respond to changes in the composition of the surrounding atmosphere with a change in conductance . This transduction mechanism of solid-state semiconducting gas sensors is normally referred to as chemo-resistive effect  and it is deepened in Chapter 1.
The first evidence about the dependence of electrical conductance from the concentration of the gases in the environment was reported in a seminal work by Brattain and Bardeen (1953) . However, the first generation of commercial devices based on SnO2 deposited via thick-film technology appeared in the sixties by Taguchi , who established the Figaro Engineering Inc.
Afterwards, chemo-resistive sensors grabbed the attention of researchers and investors with respect to different functional nanomaterials and many other techniques because this kind of sensors can be fabricated cheaply, are very compact, low-power consuming and easy to use and to implement.
The MOX sensors, can be in form of thin or thick films deposited trough screen-printing technique, spin coating, deep coating, sputtering, chemical vapor deposition, physical vapor deposition, epitaxial growth etc.. The sensing layers can be deposited onto different substrates, such as alumina, zirconia, quartz, beryllium oxide, micromachined silicon, etc.. The typical functional materials are ZnO, TiO2, SnO2, WO3, Fe2O3, LaFeO3, solid solutions as (Tix,Sn1-x)O2, added with noble metals as catalyzers or foreign ions with the role of sensitizers or conductivity modifiers, or organic molecules, functionalized graphene oxide, nanocomposites, etc..
In this work, MOX sensors are in form of thick films and they have been deposited through screen- printing technique. Indeed, the mass-production capacity (up to some hundreds of sensors at a time) at low cost with respect to other technologies, combined with devices reliability in harsh operating conditions, makes thick film planar technology particularly suitable for sensors production. They have been deposited onto alumina substrates provided with comb-type electrodes and heating elements to give to the sensor the working temperature suitable to detect the desired gas. Usually such temperature is in the range 300 – 500 °C. The functional materials must be nanosized and for this reason they have been synthesized through wet chemistry processes. The composition of the functional material, the morphology and the size at nanometric level dominate electrical and sensitivity properties of the thick films. A detailed description of the realization of sensors trough screen-printing technology is reported in Chapter 2.
Among the functional materials prepared, ZnO has been mainly investigated due to its many and various properties, synthesizing several nanostructures (nanoparticle aggregates and elongated nanocrystals).
The correlation between the obtained different morphologies and the electrical and spectroscopic behavior has been examined. Moreover ZnO gas sensors have been tested toward several reducing gases (acetone, ethanol, ammonia, etc.) typically found in exhaled human breath with the aim to use them in breath gas analysis for diagnosis of metabolic diseases. In Chapter 3, the synthesis process, the morphological, structural, spectroscopic and electrical characterizations, as well as the gas sensing properties of ZnO nanostructures are examined.
A second concrete implementation in industrial framework of the thick film gas sensors realized has been concerning the monitoring of the hydraulic oil aging. This is a novel approach (currently in patent stage) to the monitoring the aging of the hydraulic oil in real time and on-board both from a
methodological and instrumental standpoint. The same type of hydraulic oil was aged and collected using an hydraulic test bench developed at IMAMOTER-CNR and directly in a agrimotor. The oil samples have been characterized by means of gas chromatography and of a laboratory system, based on sensors, specifically prepared for this aim. It has been examined a correlation between the hydraulic oil aging and the composition of their vapors. For this application, oil samples have been also analyzed through organic electrochemical liquid sensors developed at IMEM-CNR. In Chapter 4, the oil samples collection, the methodologies used, the devices employed and the experimental results are discussed.
Finally, in Chapter 5, the description of a portable monitoring station, based on the MOX sensors, for the monitoring of traces of main atmospheric pollutant gases and some in-field experiment are came under review.
The monitoring station has been arranged, including electronics for acquisition, processing and wireless transmission of the data. A particular attention has been addressed to the development of a suitable sensor for each atmospheric pollutant gas detected (carbon monoxide, nitrogen dioxide, ozone and BTX). The in-field experiments performed during this work concerned an industrial zone in Ferrara in addition to a monitoring in Naples at monumental site of “Maschio Angioino” leaning out of an arterial road of heavy traffic close to docklands. The comparison performed between the temporal evolution of the conductivity changes of the sensors with the pollutants’ concentrations, as measured by the analytical instruments located in fixed monitoring stations managed by ARPA resulted in good agreement.
 J. S. Wilson (Ed.), Sensor technology Handbook, Elsevier Inc., 2005.
 P. Romppainen, Acta Univ. Oul C 47, 1988.
 M. J. Madou, S. R. Morrison, Chemical Sensing with Solid State Devices, New York, Academic Press, Inc., 1989.
 W. H. Brattain, J. Bardeen, Bell System Tech. J 32 (1953) 1.
 N. Taguchi, 1970 Patent specification 1280809.
SEMICONDUCTING OXIDES GAS SENSORS: EXPERIMENTAL EVIDENCES AND RESPONSE MODELING
Over the years, the demand of real time, low cost and small size devices is continuing to increase. In particular, the development of sensors for various applications ranging from micromechanics to medical diagnostics is so increased that the first decade of the 21st century has been labelled as “the sensor decade” .
The gas sensing application too is in great demand, to control a large variety of parameters such as environmental, food quality, biomedical, etc. [2-7]. In this area, recent advances in nanotechnology have been driven to an extensive investigation on semiconductor metal oxides (MOX), particularly in form of nanoceramic materials [8-11].
Sensors are devices changing almost one physical property as a result of a change of a physical or chemical property of the ambient. In particular the chemical sensors are devices changing a physical property (electrical, optical, etc.) as a result of a chemical interaction with the ambient. In this work, the sensors of interest are chemoresistive, which change their conductivity (bulk or surface) as a result of a chemical interaction with the gaseous ambient. In this frame, two categories of processes can be distinguished: i) variation in bulk conductance, which is of ionic type (it is applied the Nernst law); this type of sensors are used to control combustion processes by measuring oxygen partial pressure. The typical materials are zirconia and titania, being the working temperature greater than 700 °C; ii) variation in surface conductance is the physical quantity to measure traces of gases at constant oxygen pressure; the functional materials are metal oxides, such as SnO2, TiO2, In2O3, WO3, ZnO, LaFeO3, etc., solid solutions of them, while noble metals or foreign ions are added as catalysts or conductivity modifiers, the working temperature ranging between 200 and 500 °C.
The semiconductor oxides exhibit conductivity due to stoichiometric defects: in the ones of type n, such defects are oxygen vacancies behaving as donor levels; indeed, remaining the electrons weakly bounded, they easily enter into the conduction band. Such electrons contribute to the building of the
Schottky barrier eVs when they are captured by the acceptor surface states (in sensing materials oxygen atoms).
In a n-type semiconductor, the Schottky barrier formation occurs when the electrochemical potential at the surface is lower than that of the electrons in the conduction band. The electrons (ionized donors of the bulk) will occupy the acceptor surface states until the Fermi level will be identical in the two regions. In the diagram of the Fig. 1.1 A, the surface states are assumed neutral (acceptor states unoccupied and donor states occupied) with the Fermi level of the bulk in the middle between the bottom of the conduction band and the level of donors, while at the surface, the Fermi level is in the middle between the donor and acceptor surface states. This is an ideal case, the so-called case of “flat band”. Indeed, as reported in the Fig. 1.1 B, the electrons will occupy the acceptor surface states until an equilibrium situation will be achieved.
Fig. 1.1. Surface state bands in a semiconductor of n-type: A) flat band case; B) electron from the conduction band are captured by surface states, leading to a negatively charges surface with the counter-charge due to the positively charged donors near the surface (from Madou, Morrison, Chemical sensing with solid state devices, Academic Press Inc, San Diego, CA, 1989, p.26.).
The semiconductor oxides, differently from covalent semiconductors like silicon, prevalently exhibit ionic bonds, more localized in space and consequently more spread in energy, thus reducing the pinning effect of Fermi level . This characteristic usually allows the semiconductor oxides to be used as gas sensors; indeed, as explained later, the surface potential depends on the environmental work function.
In nanocrystalline semiconductors, the mechanism of conduction is thereby controlled by the presence of a huge series of intergranular point contacts at which a surface barrier develops, due to the presence of charged surface states. Conductance therefore is an activated process, since only those electrons with sufficient energy to cross the barrier take part to electrical conductance . The sensing mechanism is
based on the variation of the potential barrier height as a result of surface chemical reactions with environmental gases, leading to the electrical conductance modification. Such a mechanism properly works when the temperature, usually between 200 and 500 °C, is optimized with respect to both functional material and detecting gas.
Starting with this peculiar mechanism, a lot of features determine the sensor performances, but certainly the grain size reduction at nanometric level is one of the main factors enhancing their detection properties [14–16], both for large specific surface offered and for the influence in reducing the surface charge density. Indeed, when the particle dimensions scale down below a critical value, the phenomenon of the unpinning of Fermi level occurs, thus improving the sensor response of these materials . Apart from the grain size reduction, a lot of other complex factors affect the sensor performance which, in turn, is determined by the reception and transduction function along with the fabrication procedure (thin or thick film, porosity, particle agglomeration, etc.) . The selection of the functional material, the synthesis procedure, crystal size and shape, the addition of foreign elements with the role of sensitizers or conductivity modifiers are some of the factors influencing the sensor response. Understanding the mechanisms through which the sensor response is modified by each of these factors makes the semiconductor oxide suitable to be prepared with tunable physical–chemical characteristics, thus enabling the fabrication of sensor devices with specific functionality.
1.2 EXPERIMENTAL EVIDENCES
Among the above-mentioned materials, a case in point is tin dioxide, the most widely used material for gas sensing, by which in 1970 Figaro Engineering Inc. fabricated and commercialized the first metal oxide gas sensor device . SnO2 exhibits n-type semiconductor behavior due to lattice defects, in particular oxygen vacancies acting as electronic donor levels. Indeed, Samson and Fonstad experimentally determined the presence of two donor levels, Ed1 = 0.034 and Ed2 = 0.145 eV below the bottom of the conduction band . Figure 1.2 shows the Arrhenius plot obtained by changing the temperature between 360 and 900 K at the heating rate of 3 K/min (A) and the height of the surface barrier potential versus temperature (B) of a SnO2 thick-film. The direct determination of the height of the surface potential barrier at a fixed temperature is carried out using the method of temperature- stimulated conductance measurements, firstly described by Clifford and Tuma , according to which the conductance is measured as a function of time, after a change of temperature so fast that it is
possible to assume the constancy of the barrier while the conductance changes due to the variation of free carriers. Afterwards, conductance measurements were performed by changing the temperature between 300 and 900 K at the heating rate of 3 K/min. Now, through Morrison’s equation , which factorizes the surface and bulk contributions, the heights of the potential barrier as a function of temperature can be calculated from the measured conductance values. Further discussions and explanations on this point can be found in [22,23].
Fig. 1.2. Arrhenius plot (A) and energy barrier vs. temperature (B), for pure tin oxide films.
Different conductivity regions were observed, demonstrating the occurrence of different surface adsorption phenomena, in particular the O2−
– O− transformation, as experimentally proven by Chang through the correlation between electrical conductivity and EPR measurements . The typical behaviour of the SnO2 energy barrier versus temperature exhibits a minimum and a maximum corresponding to the increase of the depletion layer depth with temperature attributed to a negative surface charge accumulation, typically O− ions. The ability of tin dioxide to sense either reducing agents at high temperature or oxidizing ones, like NO2, at low temperature could be explained according to these characteristics. The interaction between the analyte and the surface of the semiconductor causes changes to the potential barrier height at the inter-granular contact and therefore to electrical conductance variations.
Passing to gas responses, Fig. 1.3 shows the SnO2 energy barriers carried out in dry air and in 500 ppm of CO in dry air. Carbon monoxide strongly affects the surface barrier height, decreasing it at all temperatures, thus demonstrating an enormous capability for SnO2 to sense CO within 200 – 400 °C.
Indeed, it means that in the phenomenon just described a great amount of electrons participates to the detection process, thus promoting the gas response. Generally, whenever it has observed a very strong response to a reducing gas, it is also highlighted this trend: a growing reducing gas response with increasing the difference between the values of the two energy barriers measured as a function of temperature.
Fig. 1.3. Energy barrier for SnO2 sample undergone to dry air (●) and to 500 ppm of CO in dry air (○).
As the first material extensively investigated in gas sensing, many studies have been performed to improve the sensing and selectivity properties of SnO2, above all by adding small amounts of noble metals on the surface [25-29]. On this matter, in the paper of Batzill and Diebold the role of additives in gas sensing materials has been deeply reviewed .
As stated above, the grain size reduction at nanometric level is one of the main factors enhancing their detection properties decreasing the grain dimension to obtain a grain size smaller than the depletion layer [12,14,31,32]. Actually, in tin oxide thick film sensors is not usual to observe the grain size dependence of the response. Indeed, the firing at high temperature causes a grain coalescence to being the grain radius up to 20-30 nm. Because the depletion layer depth in tin oxide is smaller than 20 nm, to observe this phenomenon, the sensing layers must be deposited starting from very small powders (< 10
0.4 0.5 0.6 0.7 0.8
300 400 500 600 700 800
500 ppm CO in dry air
Energy barrier [eV]
nm) and heated at moderate temperature (< 650 °C) [see next section]. Under these conditions, it was experimentally verified that the response to carbon monoxide is about twice when the grain size is about 10 nm with respect to that of a grain size of about 30 nm .
The second material to take into consideration for describing properties and behavior of metal oxide gas sensors is TiO2. The major knowledge of titania as functional material come out from catalysis and photocatalysis [34-37]. In gas sensing field, titania was initially investigated as automotive exhaust sensor for the control of the air/fuel ratio and therefore to detect oxygen, using its ionic conductivity [38-40]. Only from the nineties, titania has been studied to detect atmospheric pollutants at moderate temperature (300-600 °C) . Actually, titania is suitable to sense polluting gases in air, allowing good and stable responses, only if the grain dimension of the poly-crystalline material keeps at nanometric level. Indeed, differently from SnO2, titanium dioxide, when heated, undergoes a phase transition from anatase into rutile, simultaneously resulting in very large grain coalescence [42,43]. The anatase phase can be stabilized through the addition of ions with valence 5+ [44-46]. In particular Ta (10 at. %) allowed to hinder the transition to rutile up to 950 °C .
In spite of the excellent results in terms of anatase phase stabilization with the consequent maintenance of the grain dimension at nanometric size, the TiO2-based gas sensors differ in gas sensing behaviour from SnO2-based ones, being the latter much more reactive toward reducing gases.
Fig. 1.4 shows a comparison between the responses of samples of pure SnO2 and pure TiO2 (two sensors for each material, fired at 650 and 850 °C, respectively), to 100 ppm of CO in dry air at the working temperature of 450 °C. Two main observations can be made: i) sensing capability of SnO2 is much higher than that of titanium dioxide; ii) unlike SnO2, gas responses of titania sensors are strongly dependent on the grain size. Indeed, in SnO2 sensors the firing at 850°C is accompanied by a modest grain coalescence, as mentioned above, while in TiO2 sensors, the firing at temperatures higher than 750°C implies a crystalline phase transformation accompanied by an enormous grain coalescence, thus losing the sensing capability. TiO2 strongly differ from SnO2 also both for much smaller electrical conductivity and for the shape of the Arrhenius plot (see Fig. 1.5 A). Indeed, the sigma–shape caused in SnO2 by the occurrence of surface reactions (in particular the O2-
- O- transformation in the 200 - 400 °C range) is not visible in TiO2 because in this temperature range the donor states are not yet ionized.
Fig. 1.4. Electrical responses to 100 ppm of CO (Ggas/Gair) for two of samples of pure SnO2 and pure TiO2 (two sensors for each material, fired at 650 and 850 °C, respectively) measured at 450°C.
Fig. 1.5. Arrhenius plot for conductance (A) and energy barrier vs. temperature (B) for pure titania films
In fact, the n-type behaviour, similarly to SnO2, depends to donor-like stoichiometric defects, generally ascribed to oxygen vacancies, but with energetic positions in TiO2 much more deep inside the band gap
2 4 6 8
0 30 60 90 120 150
SN-650 SN-850 TI-650 TI-850
Time (min) G gas/G air
with respect to SnO2 [19,47]. Actually some authors assign donor levels, 0.8 eV deep, at Ti3+
ions rather than at oxygen vacancies [37,48]. Moreover titania films feature energy barriers vs temperature much higher than SnO2, where almost three activation energies are exhibited, differently from TiO2, in which only two regions of barrier are present (see Fig. 1.5 B). Both effects (shape of the barrier and intensity of gas response) are strongly related to the density of surface states, which, in turn, depends on the dimensions of the nanograins, as illustrated in the next section.
The comparison between SnO2 and TiO2 comes naturally because they exhibit the same rutile crystalline structure, space group P42/mnm, easily giving rise to a solid solution with chemical-physical properties varying with the Ti-Sn molar ratio [49,50].
Actually, the SnO2-TiO2 mixed oxide is a very interesting material for thick-film gas sensors and its synthesis and investigation (as TixSn1-xSnO2, 0 ≤ x ≤ 1) allowed to discover a completely different phenomenon occurring during the sensing process in SnO2-like materials compared with what happens in TiO2-like ones . Indeed, through FTIR analysis under CO atmosphere, for the materials with x <
0.2, as already observed in pure SnO2, a very broad absorption in the MIR region, related to the photoionization of VO˙, occurred, while samples with 0.3 ≤ x ≤ 1 exhibited a completely different phenomenon consisting in an erosion of the absorption edge related to the skeletal M–O vibration modes related to the skeletal vibration modes is observable, indicating a loss of reticular oxygen at surface during the reducing treatment. This difference of behavior, together with the definition of the phenomenon of the unpinning of the Fermi level, contributed to understand the electrical differences between SnO2 and TiO2. In , it is reported the different behavior of the samples as a result of the contribution of two detection mechanisms: i) the chemical reaction happens between the analyte and ionosorbed oxygen atoms causing an electron transfer from the surface to the bulk and vice versa in turn causing a barrier modification; ii) the oxygen atoms involved in the detection mechanism are surface lattice oxygen atoms which bond electrons that do not participate to the development of the spatial charge region and therefore of the intergranular barrier. Thus, it is reasonable that in the materials with x
< 0.3, the prevalent gas detection mechanism is the usual one (through barrier modification), whilst for x
≥ 0.3, it mainly happens through bond electrons which, after the reaction, enter CB without affecting the barrier.
In summary, with regard to the electrical properties of the various solid solutions obtained by varying the Ti molar ratio, all examined samples with 0.1 ≤ x ≤ 0.9 exhibited good sensing performance, even if they exhibited crystalline rutile structure. However, it must be noted that these materials do not undergo to phase transformation, exhibiting rutile phase as synthesized. For this reason, the grains only
moderately undergo coalescence when heated at high temperature. In Fig. 1.6, the response of the films to 50 ppm of CO (performed at the working temperature of 500°C) has been plotted together with the crystallite size of the corresponding powders heated at 1050°C,both as a function of Ti molar ratio. For both curves the best fit is a quadratic function with a correlation coefficient r2 = 0.847 for CO response, while r2 for crystallite size was 0.958.
Fig. 1.6. Response to 50 ppm of CO (performed at the working temperature of 500◦C)plotted together with the crystallite size, both as a function of Ti molar ratio.
Both phenomena are strongly dependent on the Ti molar ratio, but in the case of CO response with a greater error. Indeed, in this case two phenomena concur to the response: the content of titanium in the solid solution, but also the grain size, respect to which the dependence is linear. Looking at the CO response vs. Ti molar ratio, the material with x = 0.25 offers the highest response, being probably the material, in which the contribution to the sensing process of both mechanisms is optimized.
Other semiconductor oxides are functional materials common in gas sensing, such as WO3, ZnO, In2O3, etc., their electrical properties remaining in the range in which the Schottky barrier model for conductivity is accepted. Among them, ZnO has been pioneering material in gas sensing. Afterward it was abandoned, but recently it has met the interest of researchers as witnessed by an exponential growth of publications. Indeed, zinc oxide is a very attractive multifunctional material both for its great variety of properties and for the possibility to synthesize it in an enormous amount of nanostructures. In this work, an important part of the research activity has been devoted to the preparation and characterization
of ZnO nanostructures with a wide variety of morphologies such as nanoparticles, nanowires, nanobelts, nanorods, nanoflowers, etc., demonstrating that, in addition to the role of grain size, also the morphology can modify the electronic properties of the material, thereby having an effect onto the sensing properties.
1.3 RESPONSE MODELING
As stated above, n-type extrinsic semiconductors are characterized by the presence of free electrons in the conduction band mainly due to lattice defects, such as oxygen vacancies, generated by reducing processes during the synthesis of the material. The mechanism of conduction is controlled by electron flow through a huge series of intergranular point contacts. At these contacts a surface barrier originates in the presence of surface states, whose amount depends both on the chemical reactions with detecting gases and on the physical intrinsic characteristics of the material.
Fig. 1.7. Physical and band model for three grains of semiconductor to show how the barrier develops (A) and a TEM image of three grains of a SnO2 thick film (B).
The usual form of the Shottky barrier eVs and the corresponding potential V, is:
G. Martinelli and M.C. Carotta, Sens. and Actuators B 23 (1995) 157-161.
Madou, Morrison, Chemical sensing with solid state devices, Academic Press Inc, Sanm Diego, CA, 1989, p.37
= − ; = ( − )/
e being the absolute value of the electron charge. Wss represents the work function of the surface layer (environmental work function) and s is the electron affinity of the semiconductor.
Considering the hypotheses of the depletion approximation (DA) − applicable if the grains are much larger than the depletion layer width − : i) the total charge density equal to qNd all over the depleted region of thickness and zero elsewhere: ii) the potential Φ(r)equal to zero at the centre of the grain, as well as the electric field, and solving the Poisson equation in planar geometry:
the Schottky relation is:
where is the density of donors and (= ) the dielectric constant. The planar model, however, fails when the grain size is comparable to the extension of the depleted region Λ. In this case, indeed, it is necessary to solve the Poisson equation in spherical symmetry, since the curvature of the grain plays a relevant role. Applying the suitable boundary conditions (potential and electric field equal to zero at the centre of the grain) and imposing the grain charge neutrality, new relations for Vs and the surface state density Ns can be obtained:
r d s
(1 2 )
3 3 2
1 ( )
( ( ))
( ) 0
( ) | 0
( ) 4
r R o r R o
d o t
r r r dr
d r d r r
eN R R eN R
Solving Eq. (2) by setting the experimental values for ε, and , for particles ranging from 50 to 150 nm, it turned out that for SnO2, is almost constant. On the contrary, for TiO2 resulted in strongly decreasing as the grain radius decreased below 60 nm (see Fig. 1.8).
The traditional Schottky relation is obtained from equation 2 as Λ/R tends to zero. On the opposite limit, when R ≅ Λ, the corrective terms due to curvature, become relevant.
Fig. 1.8. Calculated density of charged surface states as a function of grain radius for SnO2 and TiO2.
This situation leads to a so-called unpinning of the Fermi level, allowing good gas responses, because the Fermi level is not forced to be at a distance from the minimum of conduction band equal to the neutral level of the surface states . Therefore, in the considered range,SnO2 cannot be considered as nanostructured, on the contrary for TiO2.
The DA, however, fails also when the free charge density current cannot be neglected. The Poisson equation must be formulated considering the complete charge density ( ) , being the second term the contribution of the mobile charge carrier at nonzero temperature:
T k r d e
r ) eN( )/
The charge density used in the DA must be achievable from this expression, in which the zero of energy (and potential) is at the bottom of the conduction band. The problem is that, in the case of powdered or polycrystalline semiconductors, the bulk can be reached only if the grain is sufficiently large. The DA
assumes, instead, that the zero-potential is always attained, independently of the grain size (see the boundary conditions for DA). This is the reason for inapplicability of the DA to small grains, for which the potential does not necessarily vanish even on the center.
The Poisson equation, considered the complete charge density, is:
ee r kBT
dr r d r
/ ) ( 2
Here the boundary conditions are slightly different from those for the DA. Because of the spherical symmetry, the condition on the field is that it vanishes on the center of the grain. For what concerns the condition on the potential, we set the zero at the bottom of the conduction band on the center of a sufficiently large grain, according to the literature. The condition of grain charge neutrality is written through the Gauss theorem.
r eN dr
Since (r) 0, when (r) is of the order of kBT, the last term could be very significant. This equation doesn’t have an analytical solution and the approximation for low values of (r) leads to the Debye length
k T / e2
Therefore, the complete extinction length of the potential is given by D. Provided that the grain radius is sufficiently large, the DA is a good approximation when is significantly larger than D. When, instead, the surface potential is small and the slope is high, the charge density used for DA is inadequate even if the radius of the grain is greater than ; this is precisely the case experimented for WO3 oxide, for which a weak dependence of conductance versus temperature reported and a low energy barrier has been measured. In this case, the depletion layer approximation doesn’t work because the condition eV S kT is not anymore satisfied.
Going back to the case of SnO2 and TiO2, using the spherical model based on the complete charge density, the difference between the two materials is evident.
Fig. 1.9. Calculated density of charged surface states as a function of grain radius for SnO2 and TiO2 in the case of numerical solution of the Poisson equation with the complete charge density.
The diagram of Fig.1.9 highlights the dependence of the density of the surface states on the grain radius both for SnO2 and TiO2, being the numerical parameters the same used in the case of depletion approximation. In SnO2, the decreasing of the surface states occurs below 20 nm, while for TiO2 it is already noticeable below 50 nm. Thereby, the two materials can be considered as nanostructured (from the point of view of the electrical conductivity) below two different critical values.
 Jon s. Wilson (Ed.), Sensor technology Handbook, Elsevier Inc., 2005.
 Kyounghoon Lee, Dae-Hyun Baek, Han-Il Jung and Jongbaeg Kim, Miniaturized VOC Detectors for Monitoring Indoor Air Quality, in C.-M. Kyung (ed.), Smart Sensors for Health and Environment Monitoring, KAIST Research Series, DOI 10.1007/978-94-017-9981-2_7.
 Inkyu Park, Daejong Yang and Kyungnam Kang, Microfabricated and Nanoengineered Chemical Sensors for Air Quality Monitoring System, in C.-M. Kyung (ed.), Smart Sensors for Health and Environment Monitoring, KAIST Research Series, DOI 10.1007/978-94-017-9981-2_6.
 S. Li, A. Simonian, and B. A. Chin, The Electrochemical Society Interface • Winter 2010
 M. Righettoni, A. Amann and S. E. Pratsinis, Breath analysis by nanostructured metal oxides as chemo-resistive gas sensors, Materials Today, Volume 18, Number 3, April 2015.
0 2 4 6 8 10 12 14 16
0 10 20 30 40 50
Grain radius (nm)
 Il-Doo Kim, Seon-Jin Choi, Sang-Joon Kim and Ji-Su Jang, Exhaled Breath Sensors, in C.-M.
Kyung (ed.), Smart Sensors for Health and Environment Monitoring, KAIST Research Series, DOI 10.1007/978-94-017-9981-2_2.
 B P J de Lacy Costello, R J Ewen and N M Ratcliffe, A sensor system for monitoring the simple gases hydrogen, carbon monoxide, hydrogen sulfide, ammonia and ethanol in exhaled breath, J.
Breath Res. 2 (2008) 037011.
 A. Ryzhikov, J. Jonca, M. Kahn, K. Fajerwerg, B. Chaudret, A. Chapelle, P. Menini, C.H. Shim, A. Gaudon, P. Fau, Organometallic synthesis of ZnO nanoparticles for gas sensing: towards selectivity through nanoparticles morphology, J. Nanopart. Res. 17(7) (2015).
 D. Lutic, M. Sanati and A. Lloyd Spetz (2007), Gas Sensors, in Rodríguez J A and Fernandez García M, Synthesis, Properties and Applications of Oxide Nanomaterials, New York, Wiley, 411- 450.
 J.G. Lu, P. Chang, Z. Fan, Quasi-one-dimensional metal oxide materials – synthesis, properties and applications, Materials Science and Engineering R 52 (2006)49–91.
 Yu-Feng Sun, Shao-Bo Liu, Fan-Li Meng, Jin-Yun Liu, Zhen Jin, Ling-Tao Kong and Jin-Huai Liu, Metal Oxide Nanostructures and Their Gas Sensing Properties: A Review, Sensors 2012, 12, 2610-2631; doi:10.3390/s120302610.
 C. Malagù, V. Guidi, M.C. Carotta, G. Martinelli, Unpinning of Fermi level innanocrystalline semiconductors, Appl. Phys. Lett. 84 (2004) 4158–4160.
 M.C. Carotta, M. Benetti, E. Ferrari, A.Giberti, C. Malagù, M. Nagliati, B. Vendemiati and G.
Martinelli, Basic interpretation of thick film gas sensors for atmospheric application, Sens.
Actuators B, 126 (2007) 672-677.
 C. Xu, J. Tamaki, N. Miura, N. Yamazoe, Grain size effects on gas sensitivity of porous SnO2- based elements, Sens. Actuators B 3 (1991) 147–155.
 X.-J. Huang, Y.-K. Choi, Chemical sensors based on nanostructured materials, Sens. Actuators B 122 (2007) 659–671.
 K.J. Choi, H.W. Jang, One-dimensional oxide nanostructures as gas-sensing materials: review and issues, Sensors 10 (2010) 4083–4099.
 N. Yamazoe, K. Shimanoe, Receptor function and response of semiconductorgas sensor, J. Sens.
 N. Taguchi, UK Patent, 1280809 (1970).
 S. Samson, C.G. Fonstad, Defect structure and electronic donor levels in stannic oxide crystals, J.
Appl. Phys. 44 (1973) 4618–4621.
 P.K. Clifford, D.T. Tuma, Characteristics of semiconductor gas sensors – II. Transient response to temperature change, Sens. Actuators 3 (83) (1982) 255–282.
 S.R. Morrison, Semiconductor gas sensors, Sens. Actuators 2 (1982) 329–341.
 V. Lantto, P. Romppainen, S. Leppävuori, A study of the temperature dependence of the barrier energy in porous tin dioxide, Sens. Actuators 14 (1988) 149–163.
 M.C. Carotta, C. Dallara, G. Martinelli, L. Passari, A. Camanzi, CH4 thick-film gas sensors:
characterization method and theoretical explanation, Sens. Actuators B 3 (1991) 191–196.
 S.C. Chang, Oxygen chemisorption on tin oxide: correlation between electrical conductivity and EPR measurements, J. Vac. Sci. Technol. 17 (1980) 366.
 N. Yamazoe, Y. Kurokawa, T. Seiyama, Effects of additives on semiconductor gas sensors, Sensors and Actuators 4 (1983) 283 – 289.
 K.D. Schierbaum, U.K. Kirner, J.F. Geiger, W. Göpel, Schottky-barrier and conductivity gas sensors based upon Pd/SnO2 and Pt/SnO2, Sensors and Actuators B 4 (1991) 87
 N. Yamazoe, New approaches for improving semiconductor gas sensors, Sensors and Actuators B 5 (1991) 7–19.
 W. Fliegel, G. Behr, J. Werner, G. Krabbes, Preparation, development of microstructure, electrical and gas-sensitive properties of pure and doped SnO2 powders, Sensors and Actuators B 18–19 (1994) 474–477.
 A. Cabot, A. Vilà, J.R. Morante, Analysis of the catalytic activity and electrical characteristics of different modified SnO2 layers for gas sensors, Sensors and Actuators B 84 (2002) 12–20.
 Matthias Batzill, Ulrike Diebold, The surface and materials science of tin oxide, Progress in Surface Science 79 (2005) 47–154.
 Noboru Yamazoe, New approaches for improving semiconductor gas sensors, Sensors and Actuators B 5 (1991) 7-19.
 Gong Zhang, Meilin Liu, Effect of particle size and dopant on properties of SnO2-based gas sensors, Sensors and Actuators B 69 (2000) 144–152.
 C. Malagù, M.C. Carotta, H. Fissan, V. Guidi, M.K. Kennedy, F.E. Kruis, G. Martinelli, T.G.G.
Maffeis, G.T. Owen, S.P. Wilks, Evidence of bandbending flattening in 10 nm polycrystalline SnO2, Sensors and Actuators B, 103 (2004) 50-54.
 S. Matsuda and A. Kato, Titanium oxide based catalysts - A review, Applied Catalysis 8 (1983) 149-165.
 Amy L. Linsebigler, Guangquan Lu, and John T. Yates, Jr., Photocatalysis on TiO2 Surfaces:
Principles, Mechanisms, and Selected Results, Chemical Reviews 95 (1995) 735-758.
 Yaron Paz, Application of TiO2 photocatalysis for air treatment: Patents’ overview, Applied Catalysis B: Environmental 99 (2010) 448–460.
 Ulrike Diebold, The surface science of titanium dioxide, Surface Science Reports 48 (2003) 53- 229.
 T.Y. Tien, H.L. Stagler, E.F. Gibbons, P.J. Zacmanidis, TiO2 as an air-to-fuel ratio sensor for automobile exhausts, Am. Ceram. Soc. Bull. 54 (1975) 280–282.
 A. Takami, Development of titania heated exhaust-gas oxygen sensor, Ceram. Bull. 67 (12) (1988) 1956– 1960.
 M.K. Akhtar, S.E. Pratsinis, S.V.R. Mastrangelo, Dopants in vapour phase synthesis of titania powders, J. Am. Ceram. Soc. 75 (1992) 3408–3416.
 H. Tang, K. Prasad, R. Sanjines, F. Levy, TiO2 anatase thin films as gas sensors. Sensors and Actuators B, 26-27 (1995) 71–75.
 R.K. Sharma, M.C. Bhatnagar, G.L. Sharma, Effect of Nb metal TiO2 oxygen gas sensor, Applied Surface Science 92 (1996) 647-650.
 M.C. Carotta, M. Ferroni, D. Gnani, V. Guidi, M. Merli, G. Martinelli, M.C. Casale, M. Notaro, Nanostructured pure and Nb-doped TiO2 as thick film gas sensors for environmental monitoring, Sensors and Actuators B 58 (1999) 310–317.
 E. Traversa, M.L. Di Vona, S. Licoccia, M. Sacerdoti, M.C. Carotta, L. Crema, G. Martinelli, Sol–
gel processed TiO2-based nano-sized powders for use in thick film gas sensors for atmospheric pollutant monitoring, J. Sol–Gel Sci. Technol. 22 (2001) 167–179.
 A.M. Ruiz, G. Dezanneau, J. Arbiol, A. Cornet, and J.R. Morante, Insights into the Structural and Chemical Modifications of Nb Additive on TiO2 Nanoparticles, Chem. Mater.16 (2004) 862-871.
 M. Sacerdoti, M.C. Dalconi, M.C. Carotta, B. Cavicchi, M. Ferroni, S. Colonna, M.L. Di Vona, XAS investigation of tantalum and niobium in nanostructured TiO2 anatase, J. Solid State Chem.
177 (2004) 1781–1788.
 S. Munnix, M. Schmeits, Origin of defect states on the surface of TiO2, Physical Review B 31 (1985) 3369-3371.
 W. Göpel, U. Kirner, H.D. Wiemhofer, Surface and bulk properties of TiO2 in relation to sensor applications, Solid State Ionics 28-30 (1988) 1423-1430.
 M. Park, T.E. Mitchell, H. Heuer, Subsolidus equilibria in the SnO2–TiO2system,J. Am. Ceram.
Soc. 58 (1) (1975) 43–47.
 T.C. Yuan, A.V. Virkar, Kinetics of spinodal decomposition in the TiO2–SnO2system: the effect of aliovalent dopants, J. Am. Ceram. Soc. 71 (1) (1988) 12–21.
 M.C. Carotta, S. Gherardi, V. Guidi, C. Malagù, G. Martinelli, B. Vendemiati, M. Sacerdoti, G.
Ghiotti, S. Morandi, Electrical and spectroscopic properties of Ti0.2Sn0.8O2 solid solution for gas sensing, Thin Solid Films 517 (2009) 6176–6183.
 M.C. Carotta, A. Fioravanti, S. Gherardi, G. Ghiotti, C. Malagù, S. Morandi, and M. Sacerdoti, (Ti, Sn) binary oxides as functional materials for gas sensing, Sensors and Actuators B 194 (2014) 195-205.
 J. Bardeen, Surface states and rectification at a metal semi-conductor contact, Phys. Rev. 71 (1947) 717.
THICK FILM PREPARATION AND CHARACTERIZATION
Thick film deposition normally is carried out through screen-printing, which is one of the oldest forms of graphic art reproduction. Screen-printing is a simple and automated manufacturing technique which allows the production of low-cost and robust chemical sensors with good reproducibility provided that the functional materials and all steps of the process are well controlled.
Thick film technology is known for hybrid circuits production, finding various applications thanks to features such compactness, robustness and, with respect to other technologies, relatively low cost. This technology is today largely applied also in the sensor field both for passive electronic components, like conductors, resistors and dielectric materials, and as primary sensors technology; among these, temperature, radiation, magnetic field, mechanical quantities and chemical sensors, the latter being the subject of this research [1,2]. The mass-production capacity (up to some hundreds of sensors at a time) at low cost with respect to other technologies, combined with devices reliability in harsh operating conditions, makes thick film planar technology particularly suitable for sensors production. Moreover, insofar as our experience is concerned, one of the main advantages of screen-printing technology for production of sensing layers is that the material preparation and film deposition can be optimized as separately. In the following, the methods to prepare and characterize the functional materials, the screen-printing deposition technique and finally the method to electrically characterize the sensing layers will be described.
2.2 PREPARATION AND CHARACTERIZATION OF THE FUNCTIONAL MATERIALS
The major requirement in developing semiconducting metal oxides for thick-film gas sensing devices is related to the control of parameters affecting the electrical properties , and in particular the sensitivity, the selectivity or cross sensitivity, meaning that the magnitude of the response to the target
gas is affected by the contemporary presence of other gases, and finally the electrical stability. Over the years, a lot of studies have been indeed addressed to improve the sensing and selectivity properties of chemoresistive gas sensors, while probably not giving the same importance to repeatability. However, thick film gas sensors, among various types of metal oxide gas sensors, are surely the most reliable provided that the base materials are prepared with suitable structural and morphological characteristics.
This particular feature, illustrated for a SnO2 based sensor, is shown in Fig. 2.1, in which the carbon monoxide concentration was alternatingly changed between 5 and 40 ppm.
Fig. 2.1. Alternate response of a SnO2-based thick film sensor to 5 and 40 ppm CO, the duration of a whole response is 1h, the duty cycle is 50%.
Thereby, the key problem of the preparation of a thick film gas sensor is the synthesis of engineered nanopowders constituting the functional materials. The chemistry is the turning point in powder- processing to obtain sensing layers with reproducible morphology (porosity, surface geometry, size of the necks,...) which take part to gas response and transduction phenomena.
Special attention is devoted to development of nanopowders with tailored characteristics via synthetic liquid-solid transformations performed under mild conditions, also called wet methods. As for any study concerning nanopowder synthesis, an accurate morphological, compositional and structural characterization of achieved products plays a very important role. Such investigations assist the
synthesis with feedback information toward the realization of material with optimal feature for gas sensing.
2.2.1 Synthesis methodology
Sol-gel methodology is a successful application of colloid science in ceramics development; it has been also chosen for its versatility to add dopants to main network of the oxide precursor. Moreover, it is suitable to prepare solid-solutions with good chemical homogeneity (i.e. non-random distribution of cations in inorganic network to be proved by further structural analyses) achieved by mixing colloidal components at low reaction temperature (T = 25-50 °C).
Two kinds of sol-gel methods can be applied: the first route involves inorganic metal salts (chlorides or nitrates) and the second one metal organic compounds, with general formula M(OR)x (R=alkyl group).
Fundamental steps are hydrolysis of the starting materials and further condensation which proceeds by olation (M-(OH)-M bonds) or oxolation (M-O-M bonds) depending on the charge density in the involved species, the metal cations determining and driving the condensation reactions.
In this work, examples of the first route are LaFeO3, WO3 and ZnO powders preparation, while examples of the second route are SnO2, TiO2, TixSn1-xO2 (0≤x≤1), SnxW1-xO2 with x = 0.1, 0.2 or 0.3 and (Ti,Ta,V)O2 solid solution.
In Fig. 2.2, a general scheme of a wet chemistry process suitable to synthesize nanostructured semiconductor oxides to use as functional materials for gas sensing is reported.
Fig. 2.2. General scheme of a “wet chemistry” process for the synthesis of semiconducting oxide powders 2.2.2 Characterization of the functional materials
X-ray diffraction - Diffraction occurs when the e-m radiation is scattered by a periodic array with long- range order, producing constructive interference at specific angles. The general condition to have diffraction is that the wavelength of the incident radiation must be similar to distance of at least two sources of diffracted waves.
X-ray diffraction (XRD) is based on the coherent elastic scattering of X-rays due to their interaction with the electrons of the material producing interference patterns. In particular, the atoms in a crystal are arranged in a periodic array and their distance is comparable to the wavelength of X-rays.
The most usual description of X-ray diffraction is known as Bragg’s model . The phenomenon is described as the selective reflection of monochromatic radiation due to the presence of crystallographic atomic planes, as shown in Fig. 2.3.
Fig. 2.3. Bragg’s law diagram.
The condition for constructive interference of an X-ray photon scattered from parallel atomic planes is described by Bragg’s equation:
where λ is the wavelength of the incident beam, dhkl is the spacing between atomic planes that generate the reflection (hkl are Miller’s indices for the single reflection), θ is the incident angle between the X- ray beam and the lattice plane and n represents the diffraction order.
During diffraction measurements the analyzed sample (thin film, powder or mono-crystal) is irradiated with a collimated monochromatic X-ray beam; the diffracted rays from the sample are then collected through a detector. The diffraction signal can be taken at different incident angles depending on the geometry adopted between source-sample-detector.
In this work, XRD analyses were performed using a Philips PW 1830 vertical powder diffractometer with Bregg–Brentano geometry (Cu Kα radiation, 40 kV, 30 mA) provided with a graphite monochromator along the diffracted beam. Diffraction patterns were collected over the range 10–120°
(2θ) with steps of 0.02° and 10 s of dwell time.
The XRD pattern contains all the structural information of a crystalline sample (space group) deducible from the angular position, the intensity and the shape of peaks. The angular position is used to determine the inter-planar distances (dhkl) and the crystallographic cell parameters, so to identify the crystalline phase univocally. The intensity of the peaks depends on the chemical composition of the examined material. The peak shape contains information about the degree of crystallinity and the strain of the sample. In general, the width of a peak is inversely proportional to the average size of crystallites along
the direction normal to the plane hkl which gives rise to that specific reflection . The crystallites size can be estimated by using Scherrer’s equation, as follows:
where βhkl is the full width at half maximum (FWHM) of the peak and K is a constant which depends on the shape of the crystallite and whose value ranges from 0.7 to 1.4.
The unit cell parameters of samples, studied in this work, were estimated through the program for Rietveld analysis (structure profile refinement) FullProf (release 2011) , while the crystallite size was estimated, according to Scherrer’s formula setting the constant K at 0.9.
Scanning Electron Microscopy, SEM - Scanning Electron Microscopy (SEM), provides information on the texture and morphology of the materials’ surface (bulk surfaces, powders or films) [7-8]. The resolution of this technique is of the order of nanometers and, when coupled with an X-rays collecting probe, allows a chemical analysis of the material's local composition. In general, a scanning electron microscope consist of an electronic source, a system of electromagnetic lenses to focus the electrons onto the sample, a vacuum system, different detectors and a computer to yield imaging and to manage the instrument. When the electron beam interacts with a material, different types of signal (electrons and X-rays) are generated (scheme in Fig. 2.4) and the image of the sample surface is reconstructed by the electronics that receive the out-coming signals from the different the detectors.
Fig. 2.4. Schematic diagram showing the regions in the interaction volume from which various types of electrons and photons originate upon irradiation with an electron beam. Adapted from .
The beam spot has variable size from a few nm to tens of nm and the area of analysis is then raster scanned and the out-coming signals are recorded as a function of the beam position to generate the image. The signals most commonly used to generate images come from secondary electrons (SE) and backscattered electrons (BSE). Secondary electrons are generated from inelastic scattering between the primary electrons (of the in-coming beam) and the electrons (from the core or the outer shells) of atoms in the sample. Such electrons have relatively low energies (< 50 eV), so it is possible to reveal only those generated in the outer layers of the material. On the contrary, all electrons with energies above 50 eV are classified as backscattered, generated as a result of elastic scattering of the electrons with the nuclei of the atoms of the material. Increasing the atomic number Z of the atoms in the sample, the contribution of backscattered electrons is strongly favored over the anelastically scattered ones.
In this work, FE-SEM (Field Emission SEM) measurements are performed using a Zeiss SIGMA (Carl Zeiss NTS GmbH, Oberkochen Germany) microscope (scheme in Fig. 2.5) equipped with a high performance Schottky field emitting source (W/ZrO2), an electron accelerator (beam booster) to minimize the effects of broadening of the beam and the optics Gemini (with “In-Lens” detector, a very high sensitivity low energy secondary electrons detector). The samples have been coated with a 10 nm layer of platinum-palladium through Ar-plasma sputtering technique to give the suitable conductivity at the samples’ surface (Quorum .Q150T-ES. Quorum Tech. Ltd., Laughton UK)
Fig. 2.5. Scheme diagram of the Zeiss SIGMA microscope column used to perform FE-SEM analysis in this work.
The SEM analysis of the samples studied in this work have been performed at ISTEC-CNR in collaboration with Dr. Mauro Mazzocchi.
IR and UV-Vis spectroscopies - IR and UV-Vis spectroscopies are suitable experimental tools to investigate the surface chemistry and the electronic properties of a wide class of metal oxides semiconductors such as those employed in this work to prepare gas sensors . When such oxides are pure and stoichiometric they behave as insulators and are transparent at middle and near infrared (MIR and NIR) radiation as well as in the UV-Visible range until the energy corresponding to the electronic transition from valence band (VB) to conduction band (CB). However, MOX semiconductors are generally characterized by a large variety of impurities and point defects, such as oxygen vacancies, which create electronic levels at different depth in the gap. For n-type semiconductor oxides, electron donor levels with energy between 0.05 and 0.5 eV can be photo-ionized by the MIR radiation (400-4000 cm-1) and the transition from the defect levels to the CB is observable. Donor levels with ionization energy > 0.5 eV correspond to NIR and Vis spectral regions. Steep absorption edge at radiation energy corresponding to the separation between defect level and the conduction band is expected. The density
of the electronic levels in the CB and the transition probability decrease on rising up in energy inside the conduction band: for this reasons, after the edge, the intensity of the absorption gradually decreases on increasing radiation frequency. The absorption edge can be made less steep if the initial level of the transition is a little band of defect levels. Moreover, in the MIR region electronic absorption edge can be modified or hidden by the presence of free electron absorption. Values of ionization energy < 0.05 eV are thermally available already at room temperature and the presence of free electrons in the CB can be revealed by a characteristic monotonic absorption (See Fig. 2.6). Truly “free” electrons cannot absorb a photon, because the requirement of energy and momentum conservation cannot be met simultaneously.
Fig.2.6. Schematic diagram showing the IR absorption bands related to free electrons in the CB (red curve) and to the transition of electrons from mono-ionized oxygen vacancies to the CB (blue curve). Adapted from .
The Vis-NIR radiation energy is usually necessary for polaronic transition, which can be described as a transition from a deep electronic level in the band gap to the CB.
Moreover, IR spectroscopy is useful to study surface reactions with gaseous species, detecting the vibrational modes of species in the gas phase or adsorbed on the surface of the sensing materials.
Indeed, in this work, IR spectroscopy has been used to study the sensing mechanism of different ZnO morphologies toward acetone. Absorption/transmission IR spectra were run on a Perkin-Elmer FTIR System 2000 spectrophotometer equipped with a Hg-Cd-Te cryo-detector, working in the range of wavenumbers 7200-580 cm-1 at a resolution of 2 cm-1. For IR analysis powder samples were compressed in self-supporting discs (10 mg cm-2) and placed in a commercial heated stainless steel cell (Aabspec) allowing thermal treatments in situ under vacuum or controlled atmosphere and the simultaneous registration of spectra at temperatures up to 600 °C. Before the measurements, the samples were treated